equal proportions has been found to be dependent on various operating parameters such as ..... 12 Michelson L D, Gideon P G, Pace E G & Kutul L H, Water.
Indian Journal of Chemical Technology Vol. 16, March 2009, pp. 136-141
Arsenic (III) removal from aqueous solutions by mixed adsorbent A P Singh, K K Srivastava & H Shekhar* *Department of Chemistry, VKS University, Ara 802 301, India Department of Chemical Engineering and Technology, Institute of Technology, Banaras Hindu University, Varanasi 221 005, India Received 28 July 2008; revised 6 January 2009 The removal of As(III) from its aqueous solutions by adsorption on homogeneous mixture of china clay and fly ash in equal proportions has been found to be dependent on various operating parameters such as concentration, temperature and pH. The As(III) removal is favourable at low concentration, high temperature and slightly basic condition at pH 8.0. The applicability of Langmuir isotherm in present system suggests the formation of monolayer coverage of As(III) molecules at the outer surface of the adsorbent. Thermodynamic parameters indicate the spontaneous and endothermic nature of the process. Adsorption kinetics studied using the model suggested by Lagergren infers a first order rate expression. Keywords: As(III) adsorption, Adsorption kinetics, China clay, Fly ash, Langmuir isotherm
Arsenic is highly toxic1-3 and is often used as herbicide and insecticide. The permissible limit of 0.06 ppm of arsenic in drinking water has been recommended by WHO and ICMR. The presence of arsenic in water beyond the permissible limit causes carcinogenic effects on living being. Its ingestion disturbs the nervous system and also acts as a casual factor for Haff’s diseasse. Acute and choronic arsenic poisoning from the consumption of arsenic contaminated drinking water have been observed. Arsenic is recognized as a cause of skin, lung and liver cancer. It is suspected of causing mouth, esophagus, larynx bladder and paranasal sinus cancer. The toxicity of arsenic varies with its oxidation state. Arsenic(III) has been reported to be more toxic than arsenic(V). Arsenic(III) exerts its toxic action by attacking –SH groups of an enzyme thereby inhibiting enzyme action. The enzyme which generate cellular energy in the citric acid cycle are adversely affected. It precipitates the proteins. Presence of arsenic in natural water may originate from effluents of pesticides and fertilizers, plant desicants, tannery operations, metallurgical industries, dyes, detergents, glassware and ceramic production. Other sources include organic and inorganic chemicals, poultry feed additives, pharmaceuticals and petroleum refining industries and rare earth industries. Arsenic is also released from smelting and roasting of mineral ores, combustion of fossils fuels, leaching of mine wastes, volcanism and land erosion. Coal and oil burning contribute about 5000 metric tones of arsenic per year.
High temperature processes involved in cement production add another approximately 3200 metric tones of arsenic per year. Among several techniques available for separation/extraction of metal ions from its solution, adsorption is preferred because of its sludge free operation and easy handling of the overall operation. In recent past much interest has been exhibited in the use of adsorption technique4 for the removal of As(III) from water and wastewater by activated carbon5 and several low cost adsorbents. In the present investigation a mixture of low cost china clay and fly ash has been used for the removal of As(III) from aquous solution by batch adsorption technique. Experimental Procedure Materials and method
China clay was obtained from Patharghatt village of Bhagalpur district of Bihar in India. Fly ash was obtained from Obra Thermal Power Plant, Mirzapur, India. Both adsorbents were sieved through 53 µm sieve and a homogeneous mixture of (1:1 ratio by weight) was obtained. The average particle size was measured by HIAC-320 Model 8002917 (ROYCO institute Division, U.S.A.). The surface area of individual and mixed adsorbents was determined by a “Three-point” N2 gas adsorption method using a model QS-7 Quantasorb Surface Area Analyzer (Quantachrome Corp., U.S.A) and the porosity was determined by Mercury Porosimeter. The density measurement was carried out using specific gravity bottle at 30°C. The chemicals used were of analytical
SINGH et al.: ARSENIC (III) REMOVAL FROM AQUEOUS SOLUTION BY MIXED ADSORBENT
reagent grade and obtained from BDH, Bombay, India. All solutions were prepared6 using distilled deionised water. Batch adsorption experiments7 were carried out by shaking 1.0 g of adsorbent mixure with 50 mL aqueous solutions of As(III) of desired concentrations at various pH and temperatures in different polythene bottles for various retention times using temperature controlled shaker at a constant speed of 220 rpm. The concentrations of As(III) remained in each sample after adsorption were determined, at desirable time intervals, by iodine monochloride method8 using a systonics UV-VIS spectrophotometer, 118 at 520 nm wavelength. Results and Discussion Main constituents of the mixed adsorbent are silica and alumina while other oxides are also present in traces, as reported earlier9. It is thus expected that most of the As(III) in aqueous medium would be removed either by alumina, silica or by a combined effect of the both oxides. Intraparticle diffusion of adsorbate species within the porses of adsorbents is also explected because of porous nature of the adsorbents. The findings of the present investigation may be discussed in the light of the following factors. Effect of concentration
The removal of As(III) by adsorption on mixed adsorbent increases with time and the equilibrium is attained in 120 min. The time of saturation (Fig. 1) is
independent of concentration of As(III). The nature of curve which is single, smooth and continuous leading to saturation suggests the possibility of formation of monolayer coverage10 on the surface of adsorbent. The arsenic uptake per unit mass of the adsorbent increases with increase in the initial concentration. However, the percentage removal increases with decrease in initial concentration. With change in concentration of As(III) from 2.5 to 10.0 ppm, the adsorbed amount increases from 0.1125 (90% removal) to 0.33 mg.g-1 (66% removal) at temperature 30°C and pH 8.0. The aqua – complexes of metal oxides present in the adsorbent are formed probably due to the chemisorption of water dipoles on the surface of adsorbent particles. These complexes are amphoteric in nature and may either dissociate proton from coordinately bonded water molecules [Eq. (1)] or may donate protons to hydroxyl ions [Eq. (2)] as follows: n+
[M (OH)n+1(OH2)m-1] +H …(1) +
[M (OH)n-1(OH2)m+1] …(2)
In the above equilibria, it is assumed that the coordination number of the metal ions remains constant. Basicity or acidity of the metal ions depends on the polarization of hydroxyl ion or, water molecules which further depends on the charge and radius of the metal ions. Adsorption kinetics
The kinetics of adsorption of As(III) on mixed adsorbent was studied in the light of Lagergren equation11: log(qe-q)=log qe-
Fig. 1 Time variation of adsorption of As(III) on China clay and fly ash mixed adsorbent at different concentrations. Conditions: particle size